This chapter will investigate the device properties of perovskite layer thicknesses using NiO or Spiro-TTB as an HTL. To compare different perovskite layer thicknesses in this section, the NiO and Spiro-TTB variants of the cell compositions introduced in section 3.2 were both utilised. An analysis was performed to quantify the influence of the thickness of the photoactive perovskite layer and to optimise the thickness for the two main hole transport layer materials. The resulting variations in the efficiency and stabilised PCE of both configurations are given in figure 5.1, and the variations in the Jsc, FF, and Voc are graphed in figure 5.2.
Figure 5.1: Efficiency and Pmppcomparison between samples with a NiO or a Spiro-TTB HTL for varying perovskite thicknesses
5.1 Thickness of the perovskite layer 57
Figure 5.2: Jsc, FF, and Voc comparison between samples with a NiO or a Spiro-TTB HTL for varying perovskite thicknesses
For the NiO HTL cells, the active area of the investigated cells is 1.04 cm2, with the exception of one 0.25 cm2 cell with a 165 nm perovskite layer for comparison. Similarly, the Spiro-TTB cells have an active area of 1.04 cm2, with the exceptions of one 165 nm and one 280 nm perovskite layer cell, both of which use 0.25 cm2.
58 5.1 Thickness of the perovskite layer
5.1.1 Analysis of NiO cells
Looking at the graph in figure 5.1a, it is evident that the layer thicknesses until 250 nm exhibit favourable efficiency behaviour, but for thicker layers there is a sudden decrease of efficiency. Figure 5.1b presents the best measured mpp tracking result of the efficiency of the cells. From 165 nm to 210 nm it is possible to obtain good mpp trackings, at 230 nm it start to become less favourable, and it has dropped off significantly at 250 nm. From this result, the carrier lifetimes are too short to allow for diffusion lengths over 230 nm, as showed by the mpp tracking.
The open circuit voltage depends on the band alignment of the cell materials, and can be improved by optimising the interfaces. It is graphed in figure 5.2a Furthermore, the fill factor (FF) is plotted in figure 5.2b. It visibly decreases before 250 nm, as it depends on the Jsc and on the Voc. Lastly, the established drop off in performance before 250 nm can also be illustrated by the sudden decrease of the short circuit current in figure 5.2c.
In conclusion, the highest short circuit current is obtained from 185 nm to 230 nm.
Furthermore, the best Voc can be obtained between 165-185 nm. The best cell obtained using the NiO HTL configuration reached an efficiency of 8.9% in mpp tracking. The size of this cell was 0.25 cm2, the FF 71.4%, the Voc 1.05 V, and the Jsc 11.7 A/m2. In the forward scan the efficiency was 8.3%, in the reverse scan it was 8.8%. Lastly, it can be noted that the cell was tested to be fully stable overnight. These results were obtained while the cell was exposed to air.
5.1.2 Analysis of Spiro-TTB cells
Similar to the case with NiO, using Spiro-TTB a trend is observed that confirms the best perovskite thickness to be from 185 nm to 200 nm. However, in contrast to the case of NiO where 165 nm was a valid thickness, for Spiro-TTB 165 nm is below the lower limit, possibly explained by a deficiency of number of carriers for a low thickness in combination with the Spiro-TTB-perovskite band alignment. Figures 5.1c and 5.1d illustrate this further, clearly showing problematic behaviour for the 165 nm and the 250 nm samples. Furthermore, the best efficiency is found around a perovskite thickness of 185-200 nm. This is observable from the mpp tracking.
Spiro-TTB theoretically has a better band alignment with high-bandgap perovskite as compared to NiO, which translates into a higher Voc value. Similar to the trend seen for the efficiency, the investigated Spiro-TTB cells exhibit the best Jsc and Voc values around 185 nm. This is depicted in figures 5.2d and 5.1f. Figure 5.2e is included as a comparison to figure 5.2b. Lastly, the tested cells had a low hysteresis at 185 nm and 200 nm.
5.1 Thickness of the perovskite layer 59
The best cell obtained using the Spiro-TTB variant of the configuration introduced in section 3.2 reached an efficiency of 7.2% in the mpp tracking. The size of this cell was 1.04 cm2, the FF 71.4%, the Voc 1.01 V, and the Jsc 12.7A/m2. In the forward scan the efficiency was 6.5%, and in the reverse scan it was 8.1%, in which a hysteresis effect is seen.
5.1.3 EQE comparison
Figure 5.3 presents a set of EQE graphs, where cells of different thickness are compared.
As stated in the figure, one compares the cells using a NiO HTL and one using a Spiro-TTB HTL. Across the two graphs, the cells with the same thickness (i.e. 165 nm, 185 nm, and 250 nm) were produced in the same batch, under the same conditions. It is apparent from the data that the Jsc attains the best values for perovskite thicknesses below 250 nm. It can be concluded that carrier extraction problems occurs at thicknesses higher than 230 nm. The recombination limit at this thickness would arise mainly because travel time across the thickness for the carriers exceeds their lifetime. Specifically, a thicker layer necessitates a longer carrier lifetime .
Figure 5.3: EQE comparison between samples with a NiO or a Spiro-TTB HTL for varying perovskite thicknesses
The EQE shape of the curves and the absorption of the perovskite layer can be juxtaposed to narrow down the location at which losses appear in the spectrum. These losses can derive from reflection or from a low absorbance of the layer at specific wavelengths. The absorbance of the NiO-perovskite substrates was plotted to investigate this further. Figure 5.4 portrays how the photon absorption increases with the thickness of the perovskite layer, especially for wavelengths between 480 nm and 650 nm.
60 5.2 Anti-reflection coating
Figure 5.4: Absorbance comparison for varying perovskite thicknesses on NiO
The light beam generated by the EQE has to pass through the glass substrate and the HTL to excite the carriers in the active area. Therefore, it should be taken into account that the reflectivity of the glass slightly lowers the obtained current. This effect will be further analysed in section 5.2.